Abstract
The elastic constant tensor of an inorganic compound provides a complete description of the response of the material to external stresses in the elastic limit. It thus provides fundamental insight into the nature of the bonding in the material, and it is known to correlate with many mechanical properties. Despite the importance of the elastic constant tensor, it has been measured for a very small fraction of all known inorganic compounds, a situation that limits the ability of materials scientists to develop new materials with targeted mechanical responses. To address this deficiency, we present here the largest database of calculated elastic properties for inorganic compounds to date. The database currently contains full elastic information for 1,181 inorganic compounds, and this number is growing steadily. The methods used to develop the database are described, as are results of tests that establish the accuracy of the data. In addition, we document the database format and describe the different ways it can be accessed and analyzed in efforts related to materials discovery and design.
Design Type(s)  observation design 
Measurement Type(s)  elastic constant tensor 
Technology Type(s)  stressstrain methodology 
Factor Type(s) 
Machineaccessible metadata file describing the reported data (ISATab format)
Background & Summary
The elastic tensor of a crystalline solid provides a complete description of its response to external forces within the elastic limit. This property is thus one of the most fundamental probes of the nature of the interatomic bonding in a given material system (e.g., ref. 1). Further, it is known that the elastic tensor correlates with many mechanical and thermal properties, and it is thus a critically important quantity for use in screening in the process of materials discovery and design. For example, since the work of Pugh in the 1950’s the ratio of the bulk to shear modulus has been used as a basis to understand and predict trends in the ductility of materials^{2–9}. More recently, extensions of the Pugh analysis have been used to derive descriptors for hardness, in the attempt to discover new materials for hard coating applications, and to guide the search for the elusive inorganic compound with a hardness greater than diamond^{3}. Elastic tensors can also be used to screen for materials with targeted thermal properties, as it provides a basis for rapid estimation of trends in heat capacities and thermal conductivities^{10–13}. Knowledge of the full anisotropic elastic tensor can be used in conjunction with mathematical homogenization theories to predict the elastic response of composite materials, and thus guide the design of such materials with targeted stiffnesses^{14,15}. Additionally, an area in which elastic properties find widespread use is geophysics, where acoustic velocities are used for interpretation of seismic data^{16,17}.
Despite the importance of the elastic tensor, experimental data for this quantity is available for only a very small subset of all known inorganic compounds. This presents a fundamental bottleneck for the discovery and design of materials with targeted thermal and mechanical properties, or for performing continuum simulations of mechanical response that require elastic moduli as input. Considering only materials for which the full tensor of elastic coefficients is available, the classical works have references that sum up to a total number of around 150 independent systems for which experimental measurements have been compiled^{18–26}. Considering papers that have investigated elastic constants of particular systems, this number might be twice as large, which is a very small fraction of the approximately 30,000 to 50,000 entries for ordered compounds in the inorganic crystal structure database^{27–29}. Among the systems for which experimental data is available are approximately 70 pure elements, with the remainder consisting of binary systems and—to a much smaller extent—ternary systems and a variety of complex minerals. Among the binary materials are solid solutions and compounds, the latter often being ordered intermetallic compounds.
One challenge associated with using published experimental data for elastic moduli is that the spread in the reported values for a given system can be quite large, depending on the details of the experimental conditions and techniques employed. For example, elastic moduli derived from inelastic neutron scattering can be 10% greater than those derived from pulseecho measurements^{30}. Differences of over 20% in reported experimental values for the bulk and shear moduli for the same system have been observed in some cases, such as NiO^{31,32}. Other experimental factors, such as different measurement temperatures^{33} and/or the presence of impurity phases, can also lead to variability in reported elastic constants.
Efforts aimed at developing databases of elastic moduli from firstprinciples computational methods have been undertaken in previous work (e.g., refs 34,35). Such a computational approach provides an advantage that all of the data can be derived in a consistent manner, facilitating comparisons across materials chemistries. In the present work we expand on this approach. Specifically, we present here the todate largest database of calculated elastic properties of crystalline inorganic compounds, ranging from metals and metallic compounds to semiconductors and insulators. These calculations are part of a highthroughput (HT) effort^{36}, undertaken within the framework of the Materials Project (MP) (www.materialsproject.org)^{37}. The database of elastic tensors currently consists of over 1,181 materials and is being updated regularly. The elastic properties are obtained using firstprinciples quantummechanical calculations based on Density Functional Theory (DFT). As shown below, the calculated elastic constants are typically within 15% of experimental values, which represents a smaller scatter than that observed in experimental values in some cases. Pearson (r) and Spearman (ρ) coefficients indicate that the calculations performed in this work yield elastic properties that show an excellent correlation with experimental values, making the database presented here useful for screening materials with properties based on elastic tensors.
The remainder of the paper is organized as follows. We first describe our method for calculating elastic constants from DFT in a HTenvironment. We then give an overview of the structure of the data, followed by a description of our results. Finally, we describe the verification and validation tests to assess the precision and accuracy of the chosen density functional and the HT algorithms employed in the calculations.
Methods
Generation of elasticity data
In this launch of the elastic constant database we tabulate results for a subset of 1,181 compounds chosen from those present in the current MP database. This subset includes 2 broad categories: i) metallic and smallbandgap compounds and ii) binary oxides and semiconductor compounds. The first category is taken from the MPdatabase, under the constraint that 1) the calculated bandgap <0.3 eV and 2) the energy above the convex hull (decomposition energy^{38}) <0.5 eV/atom. These properties have been calculated previously by DFT using the standard HTprocedure and chosen MP parameters suitable for groundstate energy, lattice structure, and band structure^{37,39}. The constraints are chosen to represent a set of materials that are metallic or nearmetallic and energetically stable or nearstable, and yields the majority of the data set (approximately 1,100 systems). For the binary oxides, different selection criteria were used: 1) the bandgap >0.3 eV and 2) the energy above the convex hull=0 eV/atom, which yields approximately 100 systems. Furthermore, approximately 20 technologically relevant semiconductors were added to create a representative set of materials.
For these systems we compute the elastic constants using a stressstrain methodology. Specifically, starting from a relaxed structure for each compound, we generate a set of distorted structures, as follows. The GreenLagrange strain tensor has 6 independent components, each of which is applied independently to every structure, with differing magnitudes, as described in the Workflow section below. For each deformed structure, the 3×3 stress tensor is calculated by DFT. If the components of the stress tensor are denoted by S_{ij} and the components of the GreenLagrange strain tensor are denoted by E_{ij}, the constitutive relation within linear elasticity can be written as in equation (1), which relates stresses to strains via the symmetric elastic matrix, with components C_{ij}. In equation (1), the following Voigtnotation is employed: $11\mapsto 122\mapsto 233\mapsto 323\mapsto 413\mapsto 512\mapsto 6$.
For each of the applied strains E_{ij}, the full stress tensor is obtained from a DFT calculation in which ionic positions are relaxed. Consequently one row (or equivalently, column) of the elastic matrix is obtained from a linear fit of the calculated stresses over the range of imposed strains. Repeating this procedure for each of the 6 independent strain components, all elements of the elastic modulus tensor can be calculated. The result is a calculated set of C_{ij} values that can be used to calculate properties such as the bulk modulus K and the shear modulus G, as described in Table 1. The components of C_{ij} depend on the choice of coordinate system and lattice vectors, and in this work we have adopted the IEEE standard^{40} for all reported tensors.
The firstprinciples results presented in this work are performed using the projector augmented wave (PAW) method^{41,42} as implemented in the Vienna Ab Initio Simulation Package (VASP)^{43,44}. In all calculations, we employ the Perdew, Becke and Ernzerhof (PBE) Generalized Gradient Approximation (GGA) for the exchangecorrelation functional^{45}. Other parameters employed in our HTDFT calculations of elastic constants are systemdependent. For the metals and metallic compounds, we employ a cutoff for the plane waves of 700 eV. Further a uniform kpoint density of approximately 7,000 per reciprocal atom (pra) is used, which means that the number of atoms per cell multiplied by the number of kpoints equals approximately 7,000. For the compounds that contain magnetic elements, a ferromagnetic state is initialized in the calculation. We expect to correctly converge to ferromagnetic and nonmagnetic states in this way, but not to antiferromagnetic states. This set of parameters results in elastic tensors that are converged to within 5% for 95% of the considered systems. Given the chemical breadth of the compound set—spanning metals, semiconductors and oxides—it is unlikely that one set of parameters performs equally well for all classes of materials. Therefore, to detect anomalies and outliers, tests were designed and corresponding firstprinciples calculations with higher convergence setting were performed (for more details see the next section). The set of approximately 20 semiconductors is calculated with the same convergence parameters as the metals and metallic compounds with similar resulting convergence. For the binary oxides, a plane wave cutoff of 700 eV is also used, with a kpoint density of 1,000 pra. This leads to elastic constants converged to within 5% for all binary oxides considered in this work. Due to the presence of strongly correlated electrons in some of the oxides, the GGA+U method is employed, with U representing the Hubbardparameter^{46,47}. The values of U are chosen consistent with those employed in the MP^{37,39}.
Workflow
In this subsection we describe the workflow for the HT implementation of the stressstrain approach to computing elastic constants described above. We note that the workflow developed for this purpose shares many features in common with that developed for elastic constantcalculations in the Vlab distributed cyberinfrastructure for materials computation^{34}. The main difference between the current approach and that described in ref. 34, is that the focus here is on elastic constants at zero pressure and temperature, whereas the Vlab workflow is developed more generally to consider elastic constants under finite pressures and temperatures, which are particularly important in the context of geophysical applications. The workflow in ref. 34 thus contains tasks related to the calculations of equations of state and finitetemperature phonon contributions, which are not considered in the present work. The emphasis here is on developing comprehensive databases of elastic moduli across a broad class of inorganic compounds, for materials design applications, and on interfacing the data with the Materials Project (MP) infrastructure.
Figure 1 summarizes the workflow for data generation implemented within the MP HT calculation infrastructure used in the present work. We start from the optimized structures in MP, and perform a tighter structural relaxation, with more stringent convergence parameters in the DFTcalculation. This initial step is necessary since the calculation of elastic constants by the stressstrain method requires a wellconverged stress tensor, and the standard HTsettings in the MP, which are optimized for the total energy, are not always sufficient for this purpose. This procedure leads to a structure exhibiting close to zero residual stresses and forces on the atoms.
The next step is to construct a set of deformed structures, for calculations of the resulting stresses. Each structure in this set is deformed homogeneously by one of the 6 independent components of the strain tensor defined above, with a magnitude chosen over a prescribed range. Similar to previous work (e.g., refs 33,48) in which a stressstrain method for computing elastic tensors has been employed, a maximum strain of 1% is applied initially to distort the structures. In our experience this value is typically large enough for most compounds to minimize the numerical noise in the calculation of the stress tensor, but small enough to remain well within the linearelastic regime. In this initial step we choose four values for the strain magnitude, varying between −1 to 1%, leading to a set of set of 24 initial deformed structures. Firstprinciples calculations of the stress tensor for each of these structures are performed, including ionic relaxations. The calculation is considered to be unsuccessful if one or more of the single deformation runs fails to converge. In such cases, the calculations are rerun with tighter numerical convergence parameters. In the case of several unsuccessful iterations, a tag to this material is generated indicating that the calculation of the elastic tensor has failed.
Once the 24 stress tensor calculations have been successfully computed, a check is performed to determine whether the range of strains considered is appropriate for deriving the elastic constant tensor using a linear stressstrain relationship. This is done by fitting the elastic constants over different ranges of strain, and examining the sensitivity of the results. We employ the following nomenclature for the chosen ranges of strains investigated: ε_{1}=(−1%, −0.5%, +0.5%, +1%), ε_{2}=(−0.5%, +0.5%), ε_{3}=(−0.75%, −0.5%, +0.5%, +0.75%), and finally ε_{4}=(−1.25%, −0.75%, +0.75%, +1.25%). We first fit the elastic constants to the default strain range, ε_{1}, and compare the resulting bulk and shear modulus to those as obtained from a fit to ε_{2}. If the results are within 15%, we move on to the next step in the workflow using the elastic constants as obtained from the fit to the strain range ε_{1}. If the discrepancies are larger than 15%, additional stress tensors are calculated for strain values of (±0.75%). We then compare the bulk and shear modulus, as fit from strain ranges ε_{2} and ε_{3}. If the results agree to within 15%, we progress in the workflow using the elastic constants as fit to the strain range ε_{2}. If again the results disagree, we compare the bulk and shear modulus, fit to ε_{1} and ε_{4}. If these agree to within 15%, we progress in the workflow using the elastic constants fit to the default strain range ε_{1}. If all of these steps fail, a warning message is generated for the compound, warranting further investigation.
From our initial set of 1,181 materials, we find that in 34 cases, either the bulk modulus and/or the shear modulus are different by over 15%, depending on whether ε_{1} or ε_{2} is used for fitting the elastic tensor. A refitting of the elastic constants of those systems is performed over the range of strains corresponding to ε_{3}, and the bulk and shear moduli are compared to those as obtained from fitting to ε_{2}. We find that only 20 systems exhibit discrepancies of over 15%. For the latter systems, we finally compare the bulk and shear moduli as obtained from fitting to ε_{1} and ε_{4}, respectively, finding that only 10 still show discrepancies of over 15%. Thus, for the vast majority of the cases considered, the default range of strains ε_{1} is found to suffice for calculations of the elastic constants by a stressstrain methodology, and for more than twothirds of the remaining compounds the additional checks implemented in the workflow lead to identification of an appropriate range of strains to yield reasonable results.
As illustrated in Fig. 1, for the systems where the calculation ends successfully and an appropriate range of strains is successfully identified, the elastic tensor results are further checked using various filters, designed to detect possible errors related to the assumption of linear elastic behavior, or other numerical inaccuracies that might occur due to the need for tighter convergence. The filters are designed to reveal physically unlikely behavior or mechanical instabilities behavior, which can be indicative of such errors. The filters include: i) K_{R} >2 GPa, ii) G_{R} >2 GPa, iii) all 6 eigenvalues of the elastic tensor are larger than zero, and iv) BornHuang stability criteria^{49} are obeyed to within a 10% margin (see below). Note that K_{R} and G_{R} represent the Reussaverages of the bulk and shear moduli, respectively^{50} (see Table 1 for definitions).
Conditions i) and ii) are selected based on an empirical observation that the most compliant known metals have shear and bulk moduli larger than approximately 2 GPa. Hence if our calculations yield results below 2 GPa for either the Reuss averages^{50} (a lower bound estimate) of K or G, these results might be correct but deserve additional attention. Condition iii) expresses the conditions for mechanical stability of solids under zero stress. If one (or more) of the eigenvalues of the elastic tensor is (are) negative, the compound is mechanically unstable at zero temperature. The effects of finite temperatures may lift the mechanical instability in some systems, such as B2 NiTi^{51}. However, negative eigenvalues may also indicate the calculation is erroneous, and hence these cases are flagged for a more detailed investigation. The final set of filters iv) is used to identify elastic tensors that correspond to materials that are mechanically stable but are near an elastic instability. This is done by applying the BornHuang elastic stability criteria for the appropriate crystal system. As an example for the cubic crystal system, we require that C_{11}−C_{12}>0, C_{11}+2C_{12}>0, C_{44}>0. If one or more of these criteria is violated, one or more of the elastic tensor eigenvalues is negative. To identify compounds that are close to a mechanical instability, we apply a small tolerance to the BornHuang criteria. As an example, for the case of cubic crystal systems, we check if C_{11}>ϵC_{12} holds true, where ϵ=1.1. We find empirically that when C_{11}<ϵC_{12}, frequently the firstprinciples calculation was not properly converged or a more accurate PAW potential is required (e.g., including semicore states). For other crystal systems, similar tests are performed.
For the materials that do not obey one or more of the conditions i)iv), we investigate the effect of the various convergence parameters in the DFT calculations, and if the results still do not pass the filters, a warning tag is generated warranting further investigation. From the initial set of 1,181 materials, it is found that 97 systems fail to meet criteria i)iv). In particular, 57 systems are found to be mechanically unstable, 16 systems have Reuss averaged shear or bulk moduli lower than 2 GPa and 19 systems are within a margin ϵ=1.1 of being mechanically unstable. For these 97 systems, a new set of calculations is performed using a substantially higher kpoint density of approximately 25,000 pra in both structural relaxations and stresscalculations. This set of calculations results in a reduction in the number of systems that do not obey conditions i)—iv) from 97 to 76 systems. Of these, 50 systems are found to be mechanically unstable, 14 systems have Reuss averaged shear or bulk moduli lower than 2 GPa and 12 systems are mechanically stable but within a margin ϵ=1.1 of being mechanically unstable. In particular, the pure metals Al and Cu are flagged by the filters in the initial DFTruns employing lower kpoints, since these metals are close to mechanical instability. However, upon increasing the kpoints, results improve (this finding was not unexpected since Cu and Al which are known to exhibit complex Fermi surfaces^{52}). The filters described above are designed to identify anomalies, and they will likely be refined as our approach evolves and additional validation is performed.
All elastic tensors that have achieved sufficient numerical convergence are inserted into the MP database and reported on the web site. We also store and report on the website results for mechanically unstable compounds, but include a warning message to the user. A JSON (JavaScript Object Notation) data document is generated for each reported elastic tensor. This JSON data document is publicly available at the Dryadrepository (Data Citation 1). We perform the structure generation and data analysis for elastic constant calculations using our opensource materials analysis code pymatgen^{53}. The workflow software FireWorks^{54} is used to automate the HT calculations and data management.
Code availability
The code for calculating elastic constants and related properties is part of the opensource code pymatgen^{53}. Pymatgen is released under the MIT (Massachusetts Institute of Technology) License and is freely accessible. The workflow as shown in Fig. 1 is powered by the opensource code FireWorks and is released under a modified GPL (GNU General Public License). Also FireWorks can be accessed and used freely.
Data Records
The calculated elastic property data and related metadata of 1,181 materials are publicly available at the Materials Project (www.materialsproject.org). The complete data set can be downloaded in a JSON (Data Citation 1) file or via the Materials Project REST API. The Materials Project also provides a convenient web interface that allows searching for materials with particular properties by querying the elastic constant database. In addition, the materials detail pages on the website now include calculated elasticity data when available.
File format
The data set for each material is stored as an individual JSON document (Data Citation 1). Based on a series of key/value pairs, the JSON format offers a readily parsable yet human readable solution for data exchange. The metadata record for each material includes descriptions of the material (e.g., structure, structure symmetry) and calculation parameters (e.g., kpoints density). The JSON keys for the metadata and their descriptions are listed in Table 2. Note that the structure is presented both in Crystallographic Information File (cif) and poscarformat. The poscarformat is the standard structure description used by the VASPcode.
Properties
The elastic constants appearing in equation (1) are calculated by DFT and represent the elastic constants of a single crystal. While singlecrystal elastic properties are important as input into higher lengthscale modeling of mechanical behavior, we also derive and report several polycrystalline averaged properties. In this work, we calculate for all considered systems the Voigt and Reuss averages of the bulk and shear modulus. The Voigt average provides an upper bound on the elastic moduli of an untextured polycrystalline material whereas the Reuss average provides a lower bound^{50}. The experimental quantities will lie between the bounds, with the precise value determined by the detailed orientation of the various grains in the material. Also we provide the empirical VRHaverage for the bulk and shear modulus. This empirical average is known to represent the bulk and shear modulus of polycrystalline materials with comparable accuracy as more advanced polycrystalline homogenization schemes such as those by Hashin and Strickman^{14,55}. Other properties computed in this work are the index of elastic anisotropy^{56} and the Poisson ratio in the isotropic approximation. The various derived properties are listed in Table 1, including expressions relating these properties to the elements of the singlecrystal elastic tensor. The corresponding JSON keys and the datatypes are also listed in Table 1. The elastic tensor C_{ij} is presented in two ways in Table 1: i) in the standardized IEEEformat and ii) in the format corresponding to the orientation of the crystal structure as defined in the poscarkey in Table 2.
Graphical representation of results
A graphical representation of our dataset is presented in Fig. 2, which shows a loglog plot of the VRH averaged bulk modulus versus the VRH averaged shear modulus for all materials considered in this work. The orientation of each arrow corresponds to the volume per atom (VPA) of that specific material. The material with the minimum VPA in our dataset is assigned an arrow pointing at 12 o’clock (diamond) and the arrows rotate anticlockwise towards the materials with the maximum VPA in our dataset at 6 o’clock (barium). The angle of rotation from 12 o’clock to 6 o’clock is proportional to the normalized VPA. The VPA is considered since it is known to correlate well with elastic properties such as bulk modulus^{57–59}. Indeed, Fig. 2 illustrates this apparent correlation. Specifically, diamond exhibits the highest bulk and shear moduli of all materials in our database and it also has the smallest VPA among those materials. The more elastically compliant materials in Fig. 2 show relatively higher values for the VPA. The color coding in Fig. 2 represents the Poisson ratio in the isotropic approximation. Also, two lines of constants K_{VRH}/G_{VRH} ratio are drawn. As described in the Introduction, this quantity, known as Pugh’s ratio^{2}, has been shown to correlate with ductility in crystalline compounds^{2,3} and is further related to the Poisson ratio^{5}. The bar plots show the distribution of materials relative to their respective values for the bulk and shear modulus. The distribution shows that most materials considered, lie in the region around 80 and 190 GPa for the shear modulus and bulk moduli, respectively. Thus, this diagram distills several wellknown results in the field of elasticity and illustrates them through a large amount of data.
Technical Validation
Verification of computational methodology
To verify proper implementation of HT version of the stressstrain method described above, detailed comparisons have been undertaken between the data derived from this approach and independent computational results obtained in the present work using alternative methods, or published previously by other authors using the same DFT approximations. Such comparisons have been undertaken for a subset of systems that are representative of the material types in the database. Overall, the comparisons yield agreement at the level of approximately 5%, with a few exceptions, as described below.
Considering first insulator compounds, the C_{ij} values obtained here for αAl_{2}O_{3} are all within 2% of the results reported in ref. 33 using the same DFT approximations, combined with a similar stressstrain method. The present αAl_{2}O_{3} results are also within 3% of the values for all C_{ij} components obtained from a numerical differentiation of the energy versus strain using Wien2K^{60,61}, and within 5% of the results for all components obtained by energy differentiation methods derived from Quantum Espresso^{62} and reported in ref. 63. It should be noted that for αAl_{2}O_{3} the C_{14} component obtained in this work has a sign opposite to that reported in ref. 63. In fact, the sign of C_{14} in αAl_{2}O_{3} has been a source of controversy in other previous theoretical and experimental studies^{33,63,64}. However, as discussed in ref. 63, the ambiguity in choosing the Cartesian reference coordinate system for trigonal materials with R centering type is the likely cause of these discrepancies. For cubic Y_{2}O_{3} the present results for each of the C_{ij} components are within 10% of those reported from the stressstrain calculations performed within GGA in ref. 64 (the largest discrepancy is found for the C_{12} component). For βSi_{3}N_{4} the present results agree to within 5% of those reported in the same publication^{64}. For the polar wurtzite ZnO compound, the results obtained in the present work agree to within 8% for C_{44}, and within 2% for all other moduli, with the values obtained by Wu et al.^{65} using the same DFT approximations, and an approach that employs densityfunctional perturbation theory to compute internal displacement contributions.
We have also conducted a number of comparisons between the present results and other theoretical calculations for metallic and smallbandgap systems. We have compared results obtained using our HT methodology with those derived from a method that fits the calculated total energy as a function of volumeconserving strains, as developed by Mehl et al.^{48,66}. The present HT stressstrain methodology yields results within 4% of those obtained from this energy versus strain method for BCC Lithium and FCC Aluminum. Further, the elastic constant tensor components for orthorhombic TiB, reported from fullpotentiallinearaugmentedplanewave GGA calculations, along with total energy differentiation methods^{67}, are within 5% for of the values obtained here for all C_{ij} components, with the exception of C_{44} (reported as C_{66} in ref. 67), which is within 15%.
As described in the previous section, consistency checks are built into the HTworkflow employed in the present work to ensure that the range of strains employed in the fit of the stressstrain relations are appropriate. The dependence of calculated elastic constants on the range of strains considered has been examined in detail in previous work, e.g., ref. 63. The authors of ref. 63 employ an energy versus strain method, using sixthorder polynomial fits of the energy to a strain range of up to 8%. The authors conclude that for small deformations, the best results are obtained by loworder polynomial fits, and that the stressstrain approach is more accurate in the sense that only firstorder derivatives are required, in which case smaller distortions are required. This is consistent with the findings in this work, where a maximum strain of 1% is found to provide reliable results for over 97% of the compounds considered, using a linear stressstrain fit. To investigate this issue further we have performed detailed tests similar to those in ref. 63 for a select number of systems. Strains in the range of 1 to 8% were applied and the stresses and strains fit using nth order polynomials, where n ranges from 1 to 4. In particular for KBr, which is one of the most elastically compliant materials in the database, we found changes of less than 2% in the bulk and shear moduli, as the strain was varied from 1 to 8%, regardless of the order of the polynomial. For diamond, the stiffest material in our database, one might expect relatively strong nonlinear behavior of the stress with strain, even for small strains. However, also for diamond we find that the bulk and shear moduli vary by less than 2% as the strain is varied and the polynomial order ranges from 1 to 4. Overall, the tests described in this and the previous section suggest that the stressstrain approach and the range of strains considered in its application, yield reliable results for the vast majority of the compounds considered in the development of the current database.
Validation through comparison to experimental measurements
A comprehensive literature review was performed to compile measured elastic constant tensors, for comparison with the present calculations, in order to establish the expected accuracy of the calculated results. In this comparison we consider only experimental sources that report the full elastic tensor, rather than only the bulk or shear modulus, so that a systematic comparison with the calculated elastic tensors can be made. In total, 104 systems are used in the comparison, including oxides and semiconductors^{18,20,23,30,32,68–74} and metals and metallic compounds^{18,20,22,26,75–79}. In the comparison, we make use of the VoigtReussHill average for K and G (denoted by K_{VRH} and G_{VRH}, respectively), which is the arithmetic mean of the Voigt and Reuss bounds^{50}. See also Table 1 for their definitions. The shear (G_{VRH}) and bulk (K_{VRH}) moduli of these 104 systems are compared by calculating the VRHaverage from the experimentally measured and calculated tensors. In addition a Euclidean difference norm^{80}, normalized by the magnitude of the calculated elastic tensor, is used to probe errors relative to the mean elastic constants: $\Vert {C}_{ij}^{exp}{C}_{ij}^{calc}\Vert \cdot {\Vert {C}_{ij}^{calc}\Vert}^{1}{\Vert {C}_{ij}\Vert}_{\mathrm{E}}={(\mathrm{tr}[{C}_{ij}^{T}{C}_{ij}])}^{0.5}$. In this expression, C_{ij} represents the elastic tensor (in matrix form) as defined in equation (1).
The comparison of calculated and experimental values for K_{VRH} and G_{VRH} are shown in Figs 3 and 4, respectively. In each plot, lines are shown indicating relative differences between computation and experiment of ±15%. As can be seen, the agreement between experiment and calculation is generally within this threshold, although there are some outliers. Specifically, in the case of the bulk modulus a discrepancy between experiment and calculations larger than 15% is found for 16 systems (in order of absolute deviation, from low to high): Na, Tl, Pb, Ca, CsI, Nd, Yb, YZn, Cd, Mg_{2}Sn, Ge, Pt, CaAl_{2}, Au, Co, CdAu. The first 11 in the list disagree with experiment by less than 10 GPa. For the shear modulus, a discrepancy between experiment and calculations larger than 15% is found for 15 systems (in order of absolute deviation, from low to high): KI, Ca, CsI, KBr, CdSe, Tl, Cd, GaSb, GaAs, Ge, CdAu, Y_{2}O_{3}, Au, Cr_{3}Si, MnSi. The first 6 in the list disagree with experiment by less than 10 GPa. These larger discrepancies may be due to errors in the calculations, the experimental measurements or a combination of both. Note that most of the systems displaying greater than 15% discrepancy between calculations and measurements are those with relatively low bulk and shear moduli, see the insets in Figs 3 and 4. Similarly, we find for the quantity $\Vert {C}_{ij}^{exp}{C}_{ij}^{calc}\Vert \cdot {\Vert {C}_{ij}^{calc}\Vert}^{1}$ most of the systems show discrepancies below 20%, with the largest discrepancies found for the systems with the smallest values of $\Vert {C}_{ij}^{calc}\Vert $. For these systems with relatively small elastic moduli, the discrepancies may be due to the larger effect of the numerical errors in the calculations on the relative precision of the calculated elastic tensors.
Other factors that might contribute to discrepancies are temperature variations: DFT provides a zerotemperature description of the state of the material, whereas many experiments are done at room temperature. While such temperature variations are typically relatively small below room temperature, in some systems this effect can be large. For example, in previous experimental studies of singlecrystal Nb_{3}Sn, the value of (C_{11}C_{12}) starts at 140 GPa and decreases to zero as temperature decreases from 300 to 32 K ref. 75. Our calculated results for Nb_{3}Sn at 0 K show a mechanical instability with C_{11} slightly less than C_{12}. Thus, these mechanical instabilities can contain useful information indicating potentially anomalous mechanical properties or shear instabilities at low temperature. Methods have been implemented in the literature to predict the temperature dependence of the elastic constants from firstprinciples^{81,82}, and implementation of such approaches represents a future extension of the database. The elastic constants reported in this work represent the zerotemperature limit of the isothermal moduli, whereas experimentally it is often the adiabatic elastic tensor that is measured; however, the differences between these two types of elastic constants are typically small^{83}. From the computational perspective, we have found that for some elements, PAW potentials exhibiting a different number of electrons as valence states can significantly affect the calculated elastic properties. This is the case for the elements V, Ti and Nb. Also, some of the systems listed above exhibit antiferromagnetic states. These states are both temperature and strain dependent, and resolving these details in HT DFTcalculations of elastic constants is challenging and the topic of current work that is expected to impact future releases of the database.
For the purpose of using the elastic constant database in the context of materials discovery, it is useful to characterize the correlation between the calculated and measured elastic quantities. For this purpose we again consider the values for K_{VRH} and G_{VRH}, and calculate the Pearson and Spearman correlation coefficients (r and ρ, respectively). Also computed are 95% bootstrapbased confidence intervals for the correlations. The lower (LB) and upper (UB) bounds of these confidence intervals are presented as ([LB, UB]). For the bulk modulus, the Pearson and Spearman correlation coefficients are 0.988 ([0.978,0.994]) and 0.988 ([0.973,0.993]), respectively. For the shear modulus, we find values of 0.994 ([0.985,0.998]) and 0.982 ([0.955,0.993]) for the Pearson and Spearman correlation coefficients, respectively. These values suggest that the measured and calculated values for bulk and shear moduli are strongly linearly associated and also, a high monotone association exists.
Usage Notes
The database presented here represents the todate largest collection of consistently calculated or measured elastic tensors for crystalline inorganic materials. We anticipate that this dataset, and the methods provided for querying it, will provide a useful tool in fundamental and applicationrelated studies of inorganic compounds. We expect, in particular, that the database will be useful for efforts aimed at materials discovery and design, in the search for and optimization of materials with targeted mechanical and thermal properties. For the first time, researchers will be able to query existing compounds from the database by specifying desired elastic properties, for example a maximum value of the shear modulus with minimum elastic anisotropy. For compounds that are currently not in the database, future extensions of this work will be a web interface where MPusers will be able to calculate elastic properties on demand, by uploading a file describing the crystallography of the material of interest. Techniques such as data mining and machine learning can be used to reveal fundamental trends in the elastic properties of compounds, and guide the screening of potentially interesting materials for target properties.
Additional information
How to cite this article: de Jong, M. et al. Charting the complete elastic properties of inorganic crystalline compounds. Sci. Data 2:150009 doi: 10.1038/sdata.2015.9 (2015).
References
References
 1
Pettifor, D. Theoretical predictions of structure and related properties of intermetallics. Mater. Sci. Technol. 8, 345–349 (1992).
 2
Pugh, S. XCII. Relations between the elastic moduli and the plastic properties of polycrystalline pure metals. Philos. Mag. 45, 823–843 (1954).
 3
Niu, H. et al. Extraelectron induced covalent strengthening and generalization of intrinsic ductiletobrittle criterion. Sci. Rep. 2, 718–723 (2012).
 4
Gschneidner, K. et al. A family of ductile intermetallic compounds. Nat. Mater. 2, 587–591 (2003).
 5
Greaves, G. N., Greer, A., Lakes, R. & Rouxel, T. Poisson’s ratio and modern materials. Nat. Mater. 10, 823–837 (2011).
 6
De Jong, M., Olmsted, D. L., van de Walle, A. & Asta, M. Firstprinciples study of the structural and elastic properties of rheniumbased transitionmetal alloys. Phys. Rev. B 86, 224101 (2012).
 7
De Jong, M., van der Zwaag, S. & Sluiter, M. Abinitio modeling of metastable precipitation processes in aluminum 7xxx alloys. Int. J. Mater. Res. 103, 972–979 (2012).
 8
Mao, Z., Chen, W., Seidman, D. N. & Wolverton, C. Firstprinciples study of the nucleation and stability of ordered precipitates in ternary AlScLi alloys. Acta Mater. 59, 3012–3023 (2011).
 9
De Jong, M. et al. Firstprinciples and genetic modelling of precipitation sequences in aluminium alloys. Solid State Phenom. 172, 285–290 (2011).
 10
Snyder, G. J. & Toberer, E. S. Complex thermoelectric materials. Nat. Mater. 7, 105–114 (2008).
 11
Cahill, D. G., Watson, S. K. & Pohl, R. O. Lower limit to the thermal conductivity of disordered crystals. Phys. Rev. B 46, 6131 (1992).
 12
Clarke, D. R. Materials selection guidelines for low thermal conductivity thermal barrier coatings. Surf. Coat. Technol. 163, 67–74 (2003).
 13
Feng, J. et al. Stability, thermal and mechanical properties of PtAl compounds. Mater. Des. 32, 3231–3239 (2011).
 14
Hashin, Z. & Shtrikman, S. A variational approach to the theory of the elastic behaviour of multiphase materials. J. Mech. Phys. Solids 11, 127–140 (1963).
 15
Zohdi, T. I. & Wriggers, P. Aspects of the computational testing of the mechanical properties of microheterogeneous material samples. Int. J. Numer. Methods Eng. 50, 2573–2599 (2001).
 16
Karki, B. B., Stixrude, L. & Wentzcovitch, R. M. Highpressure elastic properties of major materials of Earth’s mantle from first principles. Rev. Geophys. 39, 507–534 (2001).
 17
Anderson, O. L., Schreiber, E., Liebermann, R. C. & Soga, N. Some elastic constant data on minerals relevant to geophysics. Rev. Geophys. 6, 491–524 (1968).
 18
Nelson, D. LandoltBörnstein, Numerical data and functional relationships in science and technology, group III/Vol 29a (1992).
 19
Gale, W. F. & Totemeier, T. C . Smithells metals reference book. (ButterworthHeinemann, 2003).
 20
Simmons, G. & Wang, H . Single crystal elastic constants and calculated aggregate properties: a handbook (Massachusetts Institute of Technology: Cambridge, Massachusetts, 1971).
 21
Hearmon, R. F. S. The elastic constants of anisotropic materials. Rev. Mod. Phys. 18, 409 (1946).
 22
Tanaka, K. & Koiwa, M. Singlecrystal elastic constants of intermetallic compounds. Intermetallics 4, S29–S39 (1996).
 23
Nakamura, M. Elastic constants of some transitionmetaldisilicide single crystals. Metall. Mater. Trans. A 25, 331–340 (1994).
 24
Schiltz Jr., R. J. . & Smith, J. F. Elastic constants of some MAl2 single crystals. J. Appl. Phys. 45, 4681–4685 (1974).
 25
Varshni, Y. Temperature dependence of the elastic constants. Phys. Rev. B 2, 3952 (1970).
 26
Yasuda, H., Takasugi, T. & Koiwa, M. Elasticity of Nibased L12type intermetallic compounds. Acta Metall. Mater 40, 381–387 (1992).
 27
Taylor, P. Crystallographic databases edited by F. H. Allen, G. Gergerhoff and R. Sievers. Acta Crystallogr., Sect. C: Cryst. Struct. Commun. 44, 1153–1154 (1988).
 28
Belsky, A., Hellenbrandt, M., Karen, V. L. & Luksch, P. New developments in the inorganic crystal structure database (ICSD): accessibility in support of materials research and design. Acta Crystallogr., Sect. B: Struct. Sci. 58, 364–369 (2002).
 29
Setyawan, W., Gaume, R. M., Lam, S., Feigelson, R. S. & Curtarolo, S. Highthroughput combinatorial database of electronic band structures for inorganic scintillator materials. ACS Comb. Sci. 13, 382–390 (2011).
 30
Beg, M. M. & Shapiro, S. M. Study of phonon dispersion relations in cuprous oxide by inelastic neutron scattering. Phys. Rev. B 13, 1728–1734 (1976).
 31
Du Plessis, P. de V., van Tonder, S. J. & Alberts, L. Elastic constants of a NiO single crystal: I (Magnetic transitions). J. Phys. C: Solid State Phys. 4, 1983–1987 (1971).
 32
Uchida, N. & Saito, S. Elastic constants and acoustic absorption coefficients in MnO, CoO, and NiO single crystals at room temperature. J. Acoust. Soc. Am. 51, 1602–1605 (1972).
 33
Shang, S., Wang, Y. & Liu, Z.K. Firstprinciples elastic constants of α and θAl2O3. Appl. Phys. Lett. 90, 1019091:3 (2007).
 34
Da Silveira, P. R. C., da Silva, C. R. S. & Wentzcovitch, R. M. Metadata management for distributed first principles calculations in Vlaba collaborative cyberinfrastructure for materials computation. Comput. Phys. Commun. 178, 186–198 (2008).
 35
Da Silva, C. R. S. et al. Virtual laboratory for planetary materials: System service architecture overview. Phys. Earth Planet. Inter. 163, 321–332 (2007).
 36
Curtarolo, S. et al. The highthroughput highway to computational materials design. Nat. Mater. 12, 191–201 (2013).
 37
Jain, A. et al. Commentary: The Materials Project: A materials genome approach to accelerating materials innovation. APL Mater 1, 011002 (2013).
 38
Morgan, D., Ceder, G. & Curtarolo, S. Highthroughput and data mining with ab initio methods. Meas. Sci. Technol. 16, 296 (2005).
 39
The Materials Project. https://materialsproject.org/. Accessed: 20140930.
 40
IEEE standard on piezoelectricity. ANSI/IEEE Std 1761987, 0–1 (1988).
 41
Blöchl, P. E. Projector augmentedwave method. Phys. Rev. B 50, 17953–17979 (1994).
 42
Kresse, G. & Joubert, D. From ultrasoft pseudopotentials to the projector augmentedwave method. Phys. Rev. B 59, 1758–1775 (1999).
 43
Kresse, G. & Hafner, J. Ab initio molecular dynamics for liquid metals. Phys. Rev. B 47, 558–561 (1993).
 44
Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set. Phys. Rev. B 54, 11169–11186 (1996).
 45
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865 (1996).
 46
Anisimov, V. I., Zaanen, J. & Andersen, O. K. Band theory and Mott insulators: Hubbard U instead of Stoner I. Phys. Rev. B 44, 943 (1991).
 47
Dudarev, S. L., Botton, G. A., Savrasov, S. Y., Humphreys, C. J. & Sutton, A. P. Electronenergyloss spectra and the structural stability of nickel oxide: An LSDA+U study. Phys. Rev. B 57, 1505 (1998).
 48
Michael, J., Mehl, B. M. K. & Papaconstantopoulos, D. A. Intermetallic Compounds: Principles and Practice vol. 1, chap. 9 (John Wiley and Sons, 1994).
 49
Born, M. & Huang, K. Dynamical Theory of Crystal Lattices Oxford Classic Texts in the Physical Sciences (Clarendon Press: Oxford, 1988).
 50
Hill, R. The elastic behaviour of a crystalline aggregate. Proc. Phys. Soc. London, Sect. A 65, 349 (1952).
 51
Huang, X., Bungaro, C., Godlevsky, V. & Rabe, K. M. Lattice instabilities of cubic NiTi from first principles. Phys. Rev. B 65, 014108 (2001).
 52
Grabowski, B., Hickel, T., Kormann, F. & Neugebauer, J. DFTbased materials and steel design at finite temperatures. Tech. Rep. (Lawrence Livermore National Laboratory (LLNL): Livermore, CA, 2011).
 53
Ong, S. P. et al. Python materials genomics (pymatgen): A robust, opensource python library for materials analysis. Comput. Mater. Sci. 68, 314–319 (2013).
 54
Fireworks workflow software http://pythonhosted.org/FireWorks. Accessed: 20140930.
 55
Man, C.S. & Huang, M. A simple explicit formula for the VoigtReussHill average of elastic polycrystals with arbitrary crystal and texture symmetries. J. Elast. 105, 29–48 (2011).
 56
Ranganathan, S. I. & OstojaStarzewski, M. Universal elastic anisotropy index. Phys. Rev. Lett. 101, 055504 (2008).
 57
Anderson, O. L. & Nafe, J. E. The bulk modulusvolume relationship for oxide compounds and related geophysical problems. J. Geophys. Res. 70, 3951–3963 (1965).
 58
Cohen, M. L. Calculation of bulk moduli of diamond and zincblende solids. Phys. Rev. B 32, 7988 (1985).
 59
Kaxiras, E. Atomic and electronic structure of solids (Cambridge University Press, 2003).
 60
Schwarz, K. & Blaha, P. Solid state calculations using WIEN2k. Comput. Mater. Sci. 28, 259–273 (2003).
 61
Schwarz, K., Blaha, P. & Madsen, G. K. H. Electronic structure calculations of solids using the WIEN2k package for material sciences. Comput. Phys. Commun. 147, 71–76 (2002).
 62
Giannozzi, P. et al. Quantum espresso: a modular and opensource software project for quantum simulations of materials. J. Phys. Condens. Matter 21, 395502 (2009).
 63
Golesorkhtabar, R., Pavone, P., Spitaler, J., Puschnig, P. & Draxl, C. ElaSTic: A tool for calculating secondorder elastic constants from first principles. Comput. Phys. Commun. 184, 1861–1873 (2013).
 64
Yao, H., Ouyang, L. & Ching, W.Y. Ab initio calculation of elastic constants of ceramic crystals. J. Am. Ceram. Soc. 90, 3194–3204 (2007).
 65
Wu, X., Vanderbilt, D. & Hamann, D. R. Systematic treatment of displacements, strains, and electric fields in densityfunctional perturbation theory. Phys. Rev. B 72 0351051:13 (2005).
 66
Mehl, M. J. & Papaconstantopoulos, D. A. Applications of a tightbinding totalenergy method for transition and noble metals: Elastic constants, vacancies, and surfaces of monatomic metals. Phys. Rev. B 54, 4519 (1996).
 67
Panda, K. B. & Ravi Chandran, K. S. First principles determination of elastic constants and chemical bonding of titanium boride (TiB) on the basis of density functional theory. Acta Mater. 54, 1641–1657 (2006).
 68
Bond, W. L., Mason, W. P. & McSkimin, H. J. Elastic and electromechanical coupling coefficients of singlecrystal barium titanate. Phys. Rev. 82, 442–443 (1951).
 69
Lee, M. & Gilmore, R. S. Single crystal elastic constants of tungsten monocarbide. J. Mater. Sci. 17, 2657–2660 (1982).
 70
Chu, F., Lei, M., Maloy, S. A., Petrovic, J. J. & Mitchell, T. E. Elastic properties of C40 transition metal disilicides. Acta Mater. 44, 3035–3048 (1996).
 71
Sumer, A. & Smith, J. F. Elastic constants of single crystal CaMg2. J. Appl. Phys. 33, 2283–2286 (1962).
 72
Cline, C. F., Dunegan, H. L. & Henderson, G. W. Elastic constants of hexagonal BeO, ZnS, and CdSe. J. Appl. Phys. 38, 1944–1948 (1967).
 73
Son, P. R. & Bartels, R. A. CaO and SrO single crystal elastic constants and their pressure derivatives. J. Phys. Chem. Solids 33, 819–828 (1972).
 74
Ogi, H., Nakamura, N., Hirao, M. & Ledbetter, H. Determination of elastic, anelastic, and piezoelectric coefficients of piezoelectric materials from a single specimen by acoustic resonance spectroscopy. Ultrasonics 42, 183–187 (2004).
 75
Keller, K. R. & Hanak, J. J. Ultrasonic measurements in singlecrystal Nb3Sn. Phys. Rev. 154, 628–632 (1967).
 76
Wu, Y. & Hu, W. Elastic and brittle properties of the B2MgRE (RE=Sc, Y, Ce, Pr, Nd, Gd, Tb, Dy, Ho, Er) intermetallics. Eur. Phys. J. B 60, 75–81 (2007).
 77
Wang, J. et al. Firstprinciples calculations of binary Al compounds: Enthalpies of formation and elastic properties. Calphad 35, 562–573 (2011) World Round Robin Seminar 2010.
 78
Xie, Y.P., Wang, Z.Y. & Hou, Z. The phase stability and elastic properties of MgZn2 and Mg4Zn7 in MgZn alloys. Scr. Mater 68, 495–498 (2013).
 79
Shannette, G. & Smith, J. Single crystalline elastic constants of MgZn2. Scr. Metall 3, 33–35 (1969).
 80
Shahsavari, R., Pellenq, R. J.M. & Ulm, F.J. Empirical force fields for complex hydrated calciosilicate layered materials. Phys. Chem. Chem. Phys. 13, 1002–1011 (2011).
 81
Shang, S.L., Zhang, H., Wang, Y. & Liu, Z.K. Temperaturedependent elastic stiffness constants of αand θAl2O3 from firstprinciples calculations. J. Phys. Condens. Matter 22, 375403 (2010).
 82
Wu, Z. & Wentzcovitch, R. M. Quasiharmonic thermal elasticity of crystals: an analytical approach. Phys. Rev. B 83, 184115 (2011).
 83
Grimvall, G. Thermophysical properties of materials. (Elsevier, 1999).
Data Citations
 1
De Jong, M., Chen, W., Angsten, T., Jain, A., Notestine, R., Gamst, A., Sluiter, M., Krishna Ande, C., Van der Zwaag, S., Curtarolo, S., Toher, C., Plata, J., Ceder, G., Persson, K., & Asta, M. Dryad Digital Repository (2015) http://dx.doi.org/10.5061/dryad.h505v
Acknowledgements
This work was intellectually led by the Materials Project Center, supported by the BES DOE Grant No. EDCBEE. Work at the Lawrence Berkeley National Laboratory was supported by the Assistant Secretary for Energy Efficiency and Renewable Energy, under Contract No. DEAC0205CH11231. This work made use of resources of the National Energy Research Scientific Computing Center (NERSC), supported by the Office of Basic Energy Sciences of the U.S. Department of Energy under Contract No. DEAC0205CH11231.
Author information
Affiliations
Contributions
M.d.J. performed elastic constant calculations, developed the algorithm and the code and worked on data analysis and verification. W.C. performed elastic constant calculations, developed the HT implementation and worked on data analysis and verification. T.A. performed elastic constant calculations and worked on data analysis and verification. A.J. assisted in developing the code and worked on the HT implementation. R.N. performed data analysis. A.G. performed data analysis. M.S. was involved in planning the work developing the algorithm. C.A. contributed to the code and algorithm. S.v.d.Z. was involved in planning the work developing the algorithm. C.T. collaborated on the verification of the results. S.C. collaborated on the verification of the results. J.P. collaborated on the verification of the results. K.P. was involved in supervising and planning the work and its integration with the Materials Project effort. G.C. was involved in supervising and planning the work and its integration with the Materials Project effort. M.A. was involved in supervising and planning the work and its integration with the Materials Project effort. All authors contributed to the writing of the manuscript.
Corresponding author
Correspondence to Maarten de Jong.
Ethics declarations
Competing interests
The authors declare no competing financial interests.
ISATab metadata
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0 Metadata associated with this Data Descriptor is available at http://www.nature.com/sdata/ and is released under the CC0 waiver to maximize reuse.
About this article
Cite this article
de Jong, M., Chen, W., Angsten, T. et al. Charting the complete elastic properties of inorganic crystalline compounds. Sci Data 2, 150009 (2015). https://doi.org/10.1038/sdata.2015.9
Received:
Accepted:
Published:
Further reading

Metaheuristicbased inverse design of materials – A survey
Journal of Materiomics (2020)

Firstprinciples calculations of charge carrier mobility and conductivity in bulk semiconductors and twodimensional materials
Reports on Progress in Physics (2020)

Insights into the complexity of the excited states of Eudoped luminescent materials
Inorganic Chemistry Frontiers (2020)

The influence of precipitation transformation on Young's modulus and strengthening mechanism of a Cu–Be binary alloy
Materials Science and Engineering: A (2020)

The mechanical and thermodynamic properties of ZrTM (TM=Fe, Ru and Os) intermetallics under pressure and temperature: A firstprinciples predictions
Journal of Physics and Chemistry of Solids (2020)